# enhancement of quantum dot luminescence in all-dielectric metamaterial

TRANSCRIPT

arX

iv:1

210.

4146

v1 [

phys

ics.

optic

s] 1

5 O

ct 2

012

Enhancement of quantum dot luminescence in all-dielectric

metamaterial

Vyacheslav V. Khardikov∗ and Sergey L. Prosvirnin†

Institute of Radioastronomy, National Academy of Sciences of Ukraine,

4, Krasnoznamennaya Street, Kharkiv 61002, Ukraine and

School of Radio Physics, Karazin Kharkiv National University,

4, Svobody Square, Kharkiv 61077, Ukraine

Abstract

We propose a simple design of all-dielectric silicon-based planar metamaterial manifested an

extremely sharp resonant reflection and transmission in the wavelength of about 1550 nm due to

both low dissipative losses and involving a trapped mode operating method. The quality factor of

the resonance exceeds in tens times the quality factor of resonances in known plasmonic structures.

The designed metamaterial is envisioned for aggregating with a pumped active medium to achieve

an enhancement of luminescence and to produce an all-dielectric analog of a ”lasing spaser”. We

report that an essential enhancement (more than 500 times) of luminescence of layer contained

pumped quantum dots may be achieved by using the designed metamaterial. This value exceeds

manyfold the known luminescence enhancement by plasmonic planar metamaterials.

1

I. INTRODUCTION

Modern nanotechnologies effort an opportunity to structure optically thin layers of mate-

rials with a periodic subwavelength pattern in order to produce planar metamaterials. The

planar metamaterials are an impressive contemporary object, which is driven by certain

fascinating facilities both mostly well known over the decade and quite novel. Recent works

report results of aggregating laser materials with planar metamaterials to design parametric

gain systems1–3 and to develop gaining or lasing devices such as the spaser4–6. An essential

part of this development shell be the study of luminescence of an active material hybridized

with a planar metamaterial that could support a coherent high-Q electromagnetic oscillation.

Typically, a planar metamaterial assigned for visible and near infrared wavelengths is a

plasmonic structure designed on the basis of a periodic array of complex-shaped resonant

metallic nanowires or slits in a metal slab. The main factor responsible for the spectacular

properties of these metafilms is some resonant interaction of light with the patterned layer.

Moreover, numerous envisioned applications of planar metamaterials which incorporating a

pumped laser medium do require the high Q-factor resonance and a strong confinement of

electromagnetic fields.

However, losses of plasmonic metamaterials are orders of magnitude too large for the

envisioned applications. Typically, the Q-factor of the resonances excited in plasmonic

structures is small because of high radiation losses and huge energy dissipation which is

inherent to metals in the visible and near infrared wavelength ranges.

Fortunately there is a way of significantly decreasing of a radiation losses level in the

planar plasmonic structures. This way lies in using so-called ”trapped mode” resonances

observed in planar structures with broken symmetry of periodic elements due to exciting of

anti-phased currents in metallic elements of a subwavelength periodic cell in microwaves7,8

and in an optical wavelength region9–11.

Recently it was experimentally demonstrated that a hybridization of semiconductor quan-

tum dots (QDs) with a plasmonic metamaterial supported the trapped mode resonance leads

to a multifold intensity increase and narrowing of their photoluminescence spectrum12. The

experiment shows that plasmonic metamaterials interact with QDs like a cavity and lu-

minescence enhancement can be explained on base of the cavity quantum electrodynamics

Purcell effect. This observation is an essential step towards understanding the mechanism

2

of the radiation emission in plasmonic metamaterials and opens amazing possibilities for

developing metamaterial-enhanced gain artificial media.

The trapped mode resonances have a typical peak-and-trough Fano spectral profile13 and

can be excited, for example, in the planar periodic array composed of twice asymmetrically-

split metallic rings. Their specific character arises from destructive interference of the ra-

diation by the anti-phased current distribution. Theoretically, Q-factor of such resonance

can be infinitely increased by asymmetry degree decreasing in a hypothetic lossless structure

because the radiation loss level tends to zero in this case. In practice, however, in visible and

near infrared, Q-factor strongly limited by energy dissipation which is inherent to metals.

Actually, the dissipative losses increase extremely with increasing of currents in metallic ele-

ments with decrease of radiation level from nearly symmetry elements of an array. Thus the

trapped mode resonances have a larger than a regular resonance in the symmetry structure

but still moderate Q-factor11.

But there is a promising possibility to achieve a high-Q factor trapped mode resonance in

planar all-dielectric arrays with broken symmetry of practically non-dissipative elements. It

was shown in14 that using a planar array with square periodic cell consisted of two different

lengths semiconductor bars enables to achieve the trapped mode resonance with Q-factor

much larger than related to this kind of resonances in plasmonic structures. The Q-factor

of the trapped mode resonance of the germanium array can reach a value of the order of

thousand in a near infrared transparency window.

In the case of this array, the dielectric bars work as open dielectric resonators and a pair of

coupled resonators of each periodic cell may be considered as a metamolecule. The trapped

mode resonance of a planar array is formed by destructive interference of fields scattered by

such metamolecules outside of the array. Besides the large Q-factor, a remarkable property

of this resonance of all-dielectric arrays is an essential red shift of their resonant frequency

in comparison with a resonant frequency of an array which periodic cell consists of a single

dielectric bar (see14). This property opens the way for using dielectric materials with a

relatively small refractive index to produce this kind of arrays.

We can expect that a spectrum narrowing and intensity increasing of the QDs photo-

luminescence observed in12 will rise with increasing the Q-factor of the planar structure

resonance. Thus it is extremely interesting to study features of photoluminescence in a

hybridization of QDs with a periodic all-dielectric array in the trapped mode resonance

3

regime.

II. THE PROBLEM STATEMENT AND THE METHOD OF SOLUTION

Let us consider a double periodic array composed of dielectric bars placed on a substrate

with thickness Ls (see Fig. 1). The periodic array of thickness La is immersed into QD layer

(polymer layer in which QDs are dispersed) with total thickness LQD. The unit cell of the

array includes a pair of dielectric bars which have different sizes. In the paper14 asymmetry of

double periodic array of dielectric elements was obtained by using dielectric bars of identical

square cross sections but different lengths. But it is more suitable for practice using the

dielectric bars differed in width sizes along y-direction. If all bars will be identical in both

the length and the thickness then such double periodic array is very convenient for making.

The sizes of the square periodic cell are chosen dx = dy = d = 900 nm. The periodic cell is

assumed to be symmetric relatively to the line drawn through the cell center and parallel to

the y-axis. The normal incidence of a linearly x-polarized plane wave is considered.

900900

800

260

240

160

LQD

Ls

La

YX

Z

FIG. 1: (Color online) A sketch of the unite cell of the double-periodic planar structure. The

all-dielectric array composed of two dielectric bars per a periodic cell is immersed into the QD

layer.

As material for the dielectric bars we propose to use the silicon as most widespread

material of electronics which has a transparency window in the wavelength range from

4

1150 nm to 2500 nm. The sizes of the array elements are chosen to provide the trapped mode

resonance of optically non-pumped structure in wavelength 1550 nm, which is the typical

wavelength used in telecommunications. In the wavelength 1550 nm, a silicon refractive

index is approximately 3.48. Using an extremely thin substrate enables to exclude undesired

wave interference. The substrate is assumed to be a synthetic fused silica membrane. Its

refractive index is approximately ns = 1.45 in the wavelength range under consideration15.

The substrate thickness is 50 nm. It needs to notice that there are not high non-evanescent

diffraction orders in the substrate (an inequality nsd < 1550 nm is valid).

To study an intensity enhancement of the luminescence of QDs resulted from their hy-

bridization with a dielectric array we propose to use the solutions of plane wave diffraction

problem in the cases of the structure with and without optical pump. In proposed method

the photoluminescence emission intensity We is evaluated as a difference between intensity

of dissipation (or emission) defined by expression 1 − |R|2 − |T |2 in the structure without

optical pump and with it

We = W0 −W+, (1)

where W0 and W+ are intensities of dissipative losses (or emission) in the structure without

and with optical pump respectively, R and T are coefficients of reflection and transmission.

It needs to notice that the value W = 1 − |R|2 − |T |2 will be positive if a dissipation

is observed in the structure and negative in the case of a total intensity (|R|2 + |T |2) of

reflected and transmitted waves exceeds the intensity of an incident wave. This fact was

taken into account in formula (1) where the photoluminescence intensity We has a positive

value.

The proposed method was tested for validity on an example of a plasmonic metamaterial

combined with QDs which was studied experimentally in12 (see Appendix). We use the

experimental data on a luminescence spectrum presented in12 to define parameters for a

theoretical adequate description of an actual composite material which is QDs dispersed in

a host polymer layer. In additional, the comparison of experimental results of this work and

our theoretical ones give us an evidence of validity of the proposed theoretical approach to

study photoluminescence.

Thus to determine the photoluminescence intensity it is required to solve the plane wave

diffraction problem for considered structures. For this aim the mapped pseudospectral time

domain method proposed in16,17 is used. For the sake of simplicity the dispersion of dielectrics

5

is not taken into account in this paper. There are two reasons for using such approximation.

First, the dispersion of the chosen materials is very weak in the considered wavelength

range. Next this, an actual dispersion has no effect on the properties of the trapped-mode

resonances.

To take into account a gain in optically pumped QDs the method of additional differential

equations18 was used with a model of negative frequency-dependent conductivity19. The

expression of corresponding time-domain conductivity σ(t) is chosen in the form to ensure

that this value is real and causal

σ(t) =σ0

τcos(ω0t)e

−t/τu(t). (2)

Here u(t) is the Heaviside unit step function. The coefficient σ0 is proportional to the peak

value of the gain set by the pumping level and the resulting population inversion. Such model

assumes that the optical gain medium is homogeneously broadened wherein the atoms of

the gain medium are indistinguishable and have the same atomic transition frequency, ω0.

A natural variation of the QD sizes will cause the broadening of the exciton line of the QDs.

Time constant τ permits to include the relaxation processes in a phenomenological manner

(decay rate is 1/τ) and shows that any phase coherence introduced into the system of atoms

by the action of an electric field will be lost in a time interval τ once the electric field is

turned off.

The Fourier transform of σ(t) reduces to following frequency-dependent conductivity

σ(ω) =σ0/2

1 + i(ω − ω0)τ+

σ0/2

1 + i(ω + ω0)τ=

σ0(1 + iωτ)

(1 + ω20τ

2) + 2iωτ − ω2τ 2, (3)

where a time dependence of electromagnetic field is chosen in the form exp(iωt). It is clear

from (3) that the gain coefficient is governed by a single Lorentzian profile having a width

determined by τ . The resonant frequency, that is the frequency at which the response is

maximized, is given by ωd =√

ω20 + τ−2. The peak of the gain curve is σ(ωd) = σ0/2 and

the full-width-at-half-maximum bandwidth is δω = 2/τ . Using (3) one can obtain a complex

propagation constant of a plane wave and see that the wave amplification will be observed

only for the case of σ0 < 0.

The chosen form of frequency-dependent conductivity may be easily included in the cal-

culation scheme of time domain approaches by using of ADE method. It results in two

additional first order differential equations in time in each grid node immersed into the gain

medium19.

6

A good agreement of our theoretical and known experimental results of study lumi-

nescence of plasmonic metamaterial combined with QDs (see Appendix) is an evidence of

correctness both the model of active QD medium and the proposed approach to study lu-

minescence in a planar resonant metamaterial.

Now let us apply the proposed method to design a silicon resonant metamaterial com-

bined with semiconductor QDs to enhance the photoluminescence intensity with the spectral

maximum in wavelength 1550 nm.

For numerical study, a laser medium based on semiconductor QDs was chosen with fol-

lowing parameters: ω0 = 1.26 · 1015 s−1 which corresponds to wavelength λ0 = 1550 nm;

τ = 4.85 · 10−15 s; ǫQD = 2.19 which corresponds to refractive index nQD = 1.48 of non-

pumped QD laser medium, and σ0 = −500 Sm/m corresponding to an emission factor

tan δe = −0.021 on the analogy of a lossy factor of media. Small value of τ results in a

wide-band QD spectral line and it enables to exclude from consideration the effects caused

by displacement of metamaterial dissipation peak and maximum of exciton emission line of

QDs. Let us notice that the pump level (parameter σ0) is in one order less than it was need

in the case of plasmonic metamaterials (see Appendix) because of low losses of all-dielectric

array.

The geometry parameters of the dielectric bars array immersed in non-pumped QD layer

(σ0 = 0) were chosen to provide a high Q-factor trapped mode resonance of the structure

near the wavelength 1550 nm. Parameters of the silicon structure corresponding to this

condition are following La = 100 nm, LQD = 210 nm, Ls = 50 nm, length of the dielectric

bars is 800 nm, widths of bigger and smaller bars are 260 nm and 160 nm respectively, and

the distance is 240 nm between two different width bars (see Fig. 1).

To take into account the energy dissipation in dielectric bars, a model of constant con-

ductive medium was used for a description of dielectric in the PSTD method. It means that

the dielectric of bars is modeled as medium with both ǫa = n2a and σa being some constants.

Such approach results in frequency-dependent losses.

7

III. ANALYSIS OF LUMINESCENCE OF HYBRIDIZATION OF QDS WITH A

LOW-LOSS ALL-DIELECTRIC PLANAR METAMATERIAL

The wavelength dependences of reflection and transmission coefficients magnitudes of

the designed structure are shown in Fig. 2. There is a trapped mode resonance near the

wavelength 1550 nm which has the typical trough-and-peak Fano spectral profile. As it

was shown in14, this resonance results from the anti-phased excitation of the dielectric bars

operated as a half-wavelength dielectric open resonators in this case. Lines 1, 2, and 3

correspond to σa = 0, σa = 130.3 Sim/m, and σa = 1303 Sim/m or equivalently tan δa = 0,

tan δa = 10−3, and tan δa = 10−2 in the wavelength 1550 nm. Let us notice that in reality

the silicon lossy factor tan δSi is less than 10−3 in this wavelength.

1500 1520 1540 1560 1580 16000,0

0,2

0,4

0,6

0,8

1,0

|R| &

|T|

Wavelength, nm

123

|T|

|R|

FIG. 2: (Color online) Wavelength dependences of reflection and transmission coefficients of the

periodic array of silicon bars immersed in the non-pumped QD layer. Lines 1, 2, and 3 correspond

to tan δa = 0, 10−3, and 10−2 respectively.

We estimate the trapped mode resonance Q-factor by using the following formula pro-

posed in14

Q =λ1λ2

λ0|λ2 − λ1|=

2λ1λ2

|λ22 − λ2

1|, (4)

where λ1 and λ2 are wavelengths of the maximum and minimum of reflection or transmission

coefficient of corresponded Fano spectral profile and λ0 = (λ1 + λ2)/2 is an average wave-

length of the trapped mode resonance. Using (4) it was obtained following Q-factor values

8

268, 232 and 83 corresponded to tan δa = 0, 10−3 and 10−2. It is interesting that wavelength

of maximum and minimum of reflection and transmission coefficients coincide only in the

case of non-dissipative structure. Reflection and transmission extremes are shifted relatively

to each other when dissipation in dielectric taken into account and then the Q-factor of

trapped mode resonances is estimated as the average value Q = (QR + QT )/2. Here QR

and QT are calculated from wavelength dependences of reflection and transmission coeffi-

cients by formula (4). Let us notice that the average trapped mode resonant wavelength

λ0 = ((λ0)R + (λ0)T )/2 = 1551 nm is observed in all considered cases of dissipative losses.

The wavelength dependences of photoluminescence intensity We calculated by using (1)

are presented in Fig. 3. Fig. 3,a shows the photoluminescence intensity of homogeneous QD

layer which thickness is LQD = 210 nm placed on 50 nm thick silica membrane i.e. intensity

related to layered structure without any array. The wavelength dependencies of photolu-

minescence of QD hybridization with non-dissipative and low-dissipative (tan δa = 10−3)

metamaterials are presented in Fig. 3,b. One can see a large enhancement of photolumi-

nescence intensity. For the case of non-dissipative bars the photoluminescence intensity

enhances in 1560 times. If the dissipation of silicon estimated as tan δSi = 10−3 is taken into

account, this coefficient of intensity enhancement will be 560. These values are much bigger

than known orders of photoluminescence enhancement inherent to plasmonic metamaterials

combined with QDs (see12 and Appendix).

Up to this point we consider photoluminescence in the pumped all-dielectric metamaterial

with emission factor (tan δe = −0.021) which exceeds essentially in absolute value the lossy

factor of metamaterial (tan δa = 10−3). Now let us study the case of pumped lasing medium

with the intensity of energy dissipation in the dielectric array (tan δa = 10−2) is comparable

with the gain of QDs. In Fig. 4 we present wavelength dependences of the photoluminescence

intensity of QD-layer placed on silica substrate (line 1), the power dissipation in the array

of dielectric bars hybridizing with non-pumped QDs (line 2), and the photoluminescence

intensity of optically pumped QDs aggregated with the same array (line 3). In the last case

the QD photoluminescence enhancement is observed too (see Fig. 4, line 3). However, in

the trapped-mode resonance wavelength, we observe a decrease of emission intensity until

complete forbidding photoluminescence (see a grey filled region in Fig.4, where We < 0).

Such wavelength dependence of photoluminescence intensity of QDs aggregated with the

array is explained by fact that the QD gain results in an increase of field amplitude inside

9

(a)

(b)

ee

FIG. 3: (Color online) Wavelength dependences of luminescence intensity of QD layer with thick-

ness 210 nm placed on silica membrane (a), and QD layer aggregated with metamaterials (b): 1 -

tan δSi = 10−3, 2 - tan δa = 10−2.

dielectric bars and related increase of energy dissipation in the array. In the case of low

energy dissipation (for example the dissipation of silicon array with tan δSi = 10−3) this

losses result in a simple decrease of the level of photoluminescence enhancement.

10

e

FIG. 4: (Color online) Wavelength dependences of photoluminescence of QD layer with thickness

210 nm (line 1), energy absorption of QD without optical pump aggregated with array of silicon

bars (line 2) and photoluminescence of metamaterials aggregated with QD (line 3).

IV. CONCLUSIONS

We have proposed a simple design of all-dielectric silicon-based planar metamaterial man-

ifested an extremely sharp resonant reflection and transmission in the wavelength of about

1550 nm due to both low dissipative losses and involving trapped mode operating method.

Accurate numerical estimations make evidence that the quality factor of the resonance of

proposed structure exceeds in tens times the quality factor of known plasmonic structures.

The designed planar metamaterial is envisioned for aggregating with a layer of pumped

active medium to achieve an enhancement of luminescence and to produce an all-dielectric

analog of the lasing spaser5.

We have proposed an approach to study luminescence intensity of pumped QDs aggre-

gated with a planar metamaterial. The approach is based on the comparison of results of

two diffraction problems solutions. They are the problems of plane electromagnetic wave

diffraction by the structure with and without optical pump. The validity of the method has

been argued by its application to theoretical reproducing known experimental data on QD

luminescence in plasmonic metamaterials12.

We demonstrate that an essential enhancement (more than 500 times) of luminescence

intensity of layer contained pumped QDs may be achieved by using the designed all-dielectric

11

resonant metamaterial. This value exceeds manyfold the known luminescence enhancement

by plasmonic planar metamaterials.

V. ACKNOWLEDGMENTS

This work was supported by the Ukrainian State Foundation for Basic Research, Project

F40.2/037.

VI. APPENDIX

VALIDATION OF DIFFRACTION APPROACH TO STUDY LUMINESCENCE

For a validation of our approach to choosing parameters described the medium being

QDs dispersed in a host polymer and the diffraction approach to study luminescence, let

us considered one of the plasmonic metamaterials which were treated experimentally in12.

The sample consists of a gold film patterned periodically by asymmetric split-ring slits and

placed on a glass substrate (see Fig. 5). The film thickness is Lgf = 50 nm. A side size of

a square periodic cell of the array is D = 545 nm. Sizes of the slits of a periodic cell shown

in the sketch in Fig. 5 are following: a = 470 nm, t = 170 nm, and w = 65 nm. The slits

are filled with a polymer material contained semiconductor QDs and the array is coated

by a layer of the same material. The thickness of the layer is LQD = 180 nm. In12 was

used lead sulfide (PbS) semiconductor QDs from Evident Technologies with a luminescence

peak around 1300 nm and mean core diameter of 4.6 nm. These QDs were dispersed in

polymethylmethacrylate (PMMA).

Let us apply the diffraction approach based on the formula (1) to estimate the photolu-

minescence intensity of QD/PMMA hybridized with this plasmonic metamaterial.

The parameters of gain medium model must be determined before luminescence intensity

will be estimated. As it was mentioned above, the following parameters ω0, τ , and σ0

are required to determine a gain medium. Parameters ω0 and τ of QD/PMMA may be

determined from the photoluminescence peak frequency ωd =√

ω20 + τ−2 and the full-width-

at-half-maximum bandwidth of QD/PMMA photoluminescence δω = 2/τ . We use following

values ω0 = 1.47·1015 s−1 and τ = 9.69·10−15 s. Refractive index of non-pumped QD/PMMA

has the value of n = 1.48 (see12). The value of σ0 depends on level of population inversion

12

Z

Y X

LQD

t

Lgf

Ls

t

w

w

w

w

a

D D

FIG. 5: (Color online) A geometry of periodic cell of metamaterial aggregated with QD/PMMA

studied experimentally in12.

in QD/PMMA and determines the intensity of photoluminescence. Here we use the value

σ0 = −5000 Sim/m to describe an optically pumped QD/PMMA. It is a typical value which

was used to describe a gain of semiconductor media for example in19.

We consider the metamaterial aggregated with QD/PMMA placed on a semi-infinite silica

substrate (Ls → ∞). Such choosing enables us to exclude from the study the interference

in the substrate. The model of gold permittivity proposed in20 was used in our simulation

of the plasmonic metamaterial.

The results of our numerical simulation of wavelength dependences of reflection, trans-

mission, and dissipation coefficients of the metamaterial aggregated with non-pumped

QD/PMMA are shown in Fig. 6. These theoretical results may be compared with ex-

perimental ones presented in Fig. 1 of12. One can see a very good agreement between our

numerical and measured results. Some difference of levels of reflection, transmission and

absorption observed in theoretical and experimental results can be explained by distinctions

of the actual structure from the perfect periodic one.

To estimate an enhancement of luminescence intensity due to using metamaterial struc-

ture, we compare its value with the luminescence intensity of optically pumped QD/PMMA

13

FIG. 6: (Color online) Results of our numerical simulation of wavelength dependences of reflec-

tion, transmission, and dissipation coefficients of the metamaterial aggregated with non-pumped

QD/PMMA researched experimentally in12.

homogeneous layer placed on the same substrate. The thickness of the layer is chosen the

same as a total thickness of the metallic array and its QD/PMMA coating. The wavelength

dependences of photoluminescence intensity of QD/PMMA homogeneous layer which being

thickness 230 nm (line 1) and metamaterials aggregated with 180 nm-thick QD/PMMA

layer (line 2) are shown in Fig. 7. In this case we obtain 17 times enhancement of photo-

luminescence intensity. This value of luminescence enhancement exceeds only in twice the

value obtained experimentally in12 that is quite good result in modeling of active structures.

Thus, we have argued that the both our model of active QD medium and the diffraction

approach to study luminescence intensity result to numerical data being in good correspon-

dence with known measured ones.

† [email protected]; http://ri.kharkov.ua/prosvirn/

1 M. Wegener, J. L. Garcıa-Pomar, C. M. Soukoulis, N. Meinzer, M. Ruther, and S. Linden,

Optics Express 16, 19785 (2008).

2 A. Fang, T. Koschny, M. Wegener, and C. M. Soukoulis, Physical Review B 79, 241104(R)

14

e

FIG. 7: (Color online) Wavelength dependences of photoluminescence intensity of homogeneous

QD/PMMA layer (line 1) and the plasmonic metamaterial aggregated with optically pumped

QD/PMMA (line 2).

(2009).

3 Y. Sivan, S. Xiao, U. K. Chettiar, A. V. Kildishev, and V. M. Shalaev, Optics Express 17,

24060 (2009).

4 D. J. Bergman and M. I. Stockman, Phys. Rev. Lett. 90, 027402 (2003).

5 N. I. Zheludev, S. L. Prosvirnin, N. Papasimakis, and V. A. Fedotov, Nature Photonics 2, 351

(2008).

6 S. D. Campbella and R. W. Ziolkowski, Optics Communications 285, 3341 (2012).

7 S. Prosvirnin and S. Zouhdi, in Advances in Electromagnetics of Complex Media and Metamate-

rials, edited by S. Zouhdi and et al. (Kluwer Academic Publishers, Printed in the Netherlands,

2003), pp. 281–290.

8 V. A. Fedotov, M. Rose, S. L. Prosvirnin, N. Papasimakis, and N. I. Zheludev, Phys. Rev. Lett.

99, 147401 (2007).

9 S. Zhang, D. A. Genov, Y. Wang, M. Liu, and X. Zhang, Phys. Rev. Lett. 101, 047401(4)

(2008).

10 Z.-G. Dong, H. Liu, M.-X. Xu, T. Li, S.-M. Wang, S.-N. Zhu, and X. Zhang, Opt. Express 18,

18229 (2010).

11 V. V. Khardikov, E. O. Iarko, and S. L. Prosvirnin, J. Opt. 12, 045102(11) (2010).

15

12 K. Tanaka, E. Plum, J. Y. Ou, T. Uchino, and N. I. Zheludev, Phys. Rev. Lett. 105, 227403(4)

(2010).

13 U. Fano, Phys. Rev. 124, 1866 (1961).

14 V. V. Khardikov, E. O. Iarko, and S. L. Prosvirnin, J. Opt. 14, 035103(7) (2012).

15 I. H. Malitson, JOSA 55, 1205 (1965).

16 X. Gao, M. S. Mirotznik, S. Shi, and D. W. Prather, J. Opt. Soc. Am. A 21, 777 (2004).

17 V. V. Khardikov, E. O. Iarko, and S. L. Prosvirnin, Radiophysics and Radioastronomy 13, 146

(2008).

18 A. Taflove and S. C. Hagness, Computational electrodynamics: the finite-difference time-domain

method (Artech House, Boston-London, 2005).

19 R. M. J. S. C. Hagness and A. Taflove, Radio Sci. 31, 931 (1996).

20 A. Vial and T. Laroche, Appl. Phys. B 93, 139 (2008).

16